HAL Id: hal-02289822
https://hal.archives-ouvertes.fr/hal-02289822Submitted on 30 Jun 2020
HAL is a multi-disciplinary open access archive for the deposit and dissemination of sci-entific research documents, whether they are pub-lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.
Alkali-glass behavior in honeycomb-type layered
Li3-xNaxNi2SbO6 solid solution
Coélio Vallée, Matthieu Saubanère, Paula Sanz-Camacho, Yohan Biecher,
Bernard Fraisse, Emmanuelle Suard, Gwenaelle Rousse, Dany Carlier, Romain
To cite this version:
Coélio Vallée, Matthieu Saubanère, Paula Sanz-Camacho, Yohan Biecher, Bernard Fraisse, et al.. Alkali-glass behavior in honeycomb-type layered Li3-xNaxNi2SbO6 solid solution. Inorganic Chem-istry, American Chemical Society, 2019, 58 (17), pp.11546-11552. �10.1021/acs.inorgchem.9b01385�. �hal-02289822�
Alkali-glass behavior in honeycomb-type layered Li3-xNaxNi2SbO6 solid-solution
Coélio Vallée,1 Matthieu Saubanère,1,2 Paula Sanz-Camacho,2,3 Yohan Biecher 2,3 Bernard
Fraisse,1 Emmanuelle Suard,4 Gwenaëlle Rousse,2,5,6 Dany Carlier2,3, Romain Berthelot,1,2,*
1 : ICGM, Université de Montpellier, CNRS, Montpellier 34095, France
2 : Réseau sur le Stockage Électrochimique de l’Énergie (RS2E), CNRS, Amiens, France
3 : ICMCB, Université de Bordeaux, CNRS, Pessac 33608, France
4 : Institut Laue-Langevin (ILL), BP 156, 71 Avenue des Martyrs, 38042 Grenoble cedex 9, France
5 : Chimie du Solide et de l’Energie, UMR 8260, Collège de France, 11 place Marcelin Berthelot, 75231 Paris Cedex 05, France.
6 : Sorbonne Université, 4 Place Jussieu, F-75005 Paris, France
Dr. Romain Berthelot: firstname.lastname@example.org
Layered oxides compositions Li3-xNaxNi2SbO6 have been prepared by solid-state synthesis. A
complete solid-solution is evidenced and characterized by X-ray and neutron diffraction, as
well as 7Li and 23Na solid-state nuclear magnetic resonance spectroscopy. The transition metal
layer is characterized by the classic honeycomb Ni2+/Sb5+ ordering, while a more uncommon
randomly mixed occupancy of lithium and sodium is evidenced within the alkali interslab space.
In situ X-ray diffraction and DFT calculations show that this alkali disordered feature is
entropically driven. Fast cooling appears then as a synthesis root to confine bidimensional alkali
glass within crystalline layered oxides.
Graphical abstract / TOC graphic
Structural refinement and solid-state NMR validates a complete solid-solution for
honeycomb-type layered oxides Li3-xNaxNi2SbO6. An uncommon randomly mixed occupancy of lithium
Fast cooling appears then as a synthesis root to create alkali glass layer within crystalline
Ionic radii of lithium and sodium cations are significantly different in chalcogenides or halides.1
As a consequence, there are in literature very few cases of mixed lithium/sodium occupancy in
same crystallographic sites in transition metal oxides. Examples are vanadates Li1-xNaxVO32 or
bronzes LixNayV3O8, the latter being widely investigated as insertion-type negative electrode
materials for rechargeable lithium-ion batteries,3 or niobiates perovskites Li
piezoelectric properties.4–6 Regarding the important family of alkali transition metal layered
oxides, the crystallographic structure offers a large playground for solid-state chemists and
physicists due to the impressive richness of chemical compositions that can tailor different
properties. The lamellar organization is usually described by a stacking of edge-shared MO6
octahedra slabs, with intercalation of alkali ions in the interslab space. Chemical substitutions
on the transition metal layers are possible thanks to similar ionic radii in octahedral symmetry
for cations, enabling to tune some physical or chemical features. The best example might be the
emerging layered compositions LiNi1−x−yCoxAlyO2 or LiNi1−x−yMnxCoyO2 which exhibit
enhanced electrochemical performance compared to the standard electrode material LiCoO2.7– 9 On the contrary, cases of alkali ions mixed occupancy within the interslab spaces are very
scarce. To the best of our knowledge, only two examples have been reported, single crystals of
rhomboedral titanate (Na0.73Li0.24)(Li0.32Ti0.68)O2 studied by Nalbandyan,10 and nickelates
Li1-xNaxNiO2 investigated separately by Matsumura and Holzapfel in early 2000s.11–13
In the frame of discovering new layered dual-alkali transition metal layered oxides with
between Li3Ni2SbO6 and Na3Ni2SbO6 (or LiNi2/3Sb1/3O2 and NaNi2/3Sb1/3O2, respectively).
These compounds are structurally related to O3-type14 LiCoO2, with an additional
honeycomb-type ordering of the Ni2+ and Sb5+ cations.15–18 A complete solid-solution could be obtained by
ceramic route one-pot synthesis from carbonates or oxides precursors. The lithium/sodium
mixed occupancy is confirmed by structural refinement and solid-state NMR spectroscopy. The
alkali ions random distribution is not thermodynamically stable as decomposition is observed
by in situ XRD during either heating or slow cooling. These results pave the way to design
crystalline layered compounds with 2D confined alkali glass.
Li3Ni2SbO6, Na3Ni2SbO6 and intermediate compositions Li3-xNaxNi2SbO6 (0 ≤ x ≤ 3) have
been prepared by conventional solid-state synthesis. Dried alkali carbonates (Li2CO3, Aldrich,
99.997 % or Na2CO3, Sigma-Aldrich, 99.5 %) are thoroughly mixed with nickel and antimony
oxides (NiO, Prolabo and Sb2O3, Merck, 99 %), with a nominal alkali excess of 5-10 wt.% to
compensate the high-temperature volatility. The resulting mixtures are then pelletized and
heated for 5 hours at 900 °C in air on a platinum crucible. A rapid quench in oil bath ends the heat treatment, and the resulting pellets are then washed with ethanol and dried before storage.
X-ray diffraction (XRD) was performed on a Bruker D8 Discovery diffractometer with Kα1 Cu
radiation, from 5 to 120 ° (16 h of total scan). Sample powders were sieved below 100 µm for
analysis. Moreover, the thermal stability of the samples was followed in situ by XRD on a PANalytical Empyrean with Kα Co radiation and equipped with an Anton Paar heating
Neutron powder diffraction (ND) was carried out at room temperature out at Institut Laue
as-prepared powder of the composition Li1.5Na1.5Ni2SbO6 have been sealed in a cylindrical
23Na MAS NMR spectra were recorded on a Bruker 300 Avance spectrometer at 79.49 MHz
(7.05 T magnet) using a standard Bruker 2.5 MAS probe at a spinning frequency of 30 kHz and
a recycle time D0 = 0.5 s, long enough to avoid T1 saturation effects. A one rotor period
synchronized Hahn echo sequence was used with a 90° pulse length of 1.5 µs. The external
reference was a 1 mol.L-1 NaCl aqueous solution. 7Li MAS NMR spectra were recorded on a
Bruker Avance III spectrometer at 38.93 MHz (2.35 T magnet), a standard Bruker 2.5 MAS
probe at a 30 kHz spinning frequency. A Hahn echo sequence was used with a 90° pulse of
1.6 µs with a relaxation time of 1 s. The 0 ppm external reference was a 1 M LiClaqueous
Density functional theory calculation (DFT+U) used the monoclinic description of Zvereva18
with two alkali layers (C 2/m space group) as starting point. About hundred different
crystallographic structures have been generated with a random distribution of lithium and
sodium ions over the 24 available positions. All structures have been fully relaxed using the plane wave code “Vienna Ab-Initio Simulation Package” with PAW pseudo-potentials and the
PBE functional.19–21 A Ueff = 4 eV is considered to take into account electron-electron
interactions on nickel.22 The forces on the atoms were converged to 5 10-3 eV/Å with a
Results and Discussion
An alkali ions mixed occupancy
XRD patterns obtained with a final quenching at the end of the thermal treatment are gathered
in Figure 1a for all compositions from Li3Ni2SbO6 to Na3Ni2SbO6. No extra peak could be
assigned to impurities like binary oxides or alkali hydroxides, and the patterns could be indexed
using the monoclinic symmetry (space group C 2/m). In comparison with a classic O3-type stacking (α-NaFeO2 polytype), the Ni2+/Sb5+ honeycomb ordering induces superstructure peaks
visible in the 19 – 32 ° 2θ region. They can be nicely observed in Figure 1b, with for Li-rich
compositions a broadening that is reminiscent of stacking faults, as commonly observed in such
honeycomb-ordered lamellar oxides.15–17
The refined cell parameters evolve regularly all along the chemical compositions, following a classical Vegard’s law (Figure S1). The evolution of the corresponding monoclinic cell volume
shown in inset of Figure 1c demonstrates a complete solid-solution behavior from Li3Ni2SbO6
to Na3Ni2SbO6. The question arising from this assumption is the localization of both lithium
and sodium cations. Three structural models seem possible. They are pictured in Figure 2 for
the particular compositions Li1.5Na1.5Ni2SbO6. The first one is a mixed occupancy of lithium
and sodium ions and a random in-plane distribution within. Following the structural description
of Zvereva18 and Ma17, the slab thickness (basically including one transition metal and one
alkali layers) is 4.856 Å and 5.344 Å for Li3Ni2SbO6 and Na3Ni2SbO6. From lithium-rich to
sodium-rich end members, the increase is about 10 % and comes from an important
enhancement of the alkali layer (from 2.60 Å to 3.21 Å, hence + 23.5 %) whereas the transition
metal layer is slightly contracted. In our case, the linear evolution of the slab thickness also
shows an increase of about 10 % (Figure 1d) and consequently supports this structural
In the second model, lithium and sodium ions always occupy the same interslab space but
following an in-plane ordering (either chains, stripes, cluster, etc.). The last model also lies on
alkali ions ordering, lithium and sodium ions occupy distinct interslab spaces. For the
intermediate composition Li1.5Na1.5Ni2SbO6, such arrangement would result in alternate
Li+/Na+ layers, as it has been already evidenced for the unique case of OP4-LixNayCoO2.23 It is
important to point out that, in the two latter models, the mean slab thickness evolution
(determined from the out-of-plane c parameter) could be also assumed.
In alkali transition metal layered oxides, alkali cations out-of-plane ordering like in
OP4-LixNayCoO2 or alkali cations / vacancies in-plane ordering like in Na1/2CoO2 or K4/7CoO2
lead to significant superstructure peaks in X-ray diffraction pattern.23–25 The two last
abovementioned models involve cationic ordering and the corresponding simulated patterns
clearly evidence superstructure peaks (Figure S2). The absence of such peak in our
high-resolution XRD pattern in Figure 1 is a first clue to discard these two hypotheses and
consequently to support the model of random Li/Na distribution despite their different ionic
radii (0.76 and 1.02 Å in octahedral symmetry, respectively).1
In order to get local information on lithium and sodium environments, solid-state NMR has
been further carried out for all the compositions, and corresponding 7Li and 23Na spectra are
shown in Figure 3. The peak shifts for all compounds results from the Fermi contact interaction
between the paramagnetic low spin Ni2+ (t2g6eg2) ions and the probed nucleus. This interaction
occurs through the chemical bonds and therefore denotes the local electronic structure.
Whatever the structural hypotheses presented above, the two alkaline A+ ions in the system are
surrounded by four Ni2+ as first cation neighbors (90° A-O-Ni interaction) and four Ni2+ as
For Li3Ni2SbO6, two distinct narrow peaks at 492 and 420 ppm and a larger set of signals around
300 ppm are observed by 7Li MAS NMR. According to the literature, based on their relative
intensities, the two first are assigned to lithium ions respectively in 2d and 4h Wyckoff positions
of the space group C 2/m, i.e. within the interslab space in octahedral insertion sites. The third
broad contribution around 300 ppm could be assigned to stacking defects, similarly to stacking
faults observation in the Li2MnO3 reported by Grey and coworkers.26 Indeed, the relative
intensity of the contribution at 300 ppm compared to the two other sharp peaks depends on the
synthesis conditions: when Li3Ni2SbO6 is prepared with a final slow cooling, the two first peaks
are clearly sharper and the broad contribution almost disappear (Figure S3). On the opposite
side of the Figure 3, 23Na NMR spectrum for Na3Ni2SbO6 exhibits two contributions located at
1440 ppm and 1300 ppm with no second order quadrupolar lineshape, contrary to the spectrum
reported by Ma et al. using a lower magnetic field (200 MHz spectrometer) and a higher
spinning frequency (50 KHz).17 Based on the relative peak intensities, we can also assign those
two peaks to Na ions in the in 2d and 4h sites respectively. Interestingly, the difference between
quenched and non-quenched Na3Ni2SbO6 is very weak as both XRD pattern and NMR data
look very similar (Figure S4). Thanks to higher weight and larger ionic radii of sodium compare
to lithium and in agreement with the observation of superstructure peaks shapes in inset of
Figure 1, Na3Ni2SbO6 seems to ordered more easily than Li3Ni2SbO6 and is therefore less
sensitive to quenching.
Intermediate compositions Li3-xNaxNi2SbO6 can be analyzed by both 7Li and 23Na NMR. At a
first glance, broader resonance peaks are clearly evidenced. In both cases, the broadness
increases when compositions moves away from Li3Ni2SbO6 or Na3Ni2SbO6. Moreover, a weak
but significant peak shift also accounts for variation of the (Li – O and Na – O) interatomic
distances. Shifting toward lower ppm in 7Li NMR spectra corresponds to a decrease of the
the Li – O distances, whereas displacement to higher ppm in 23Na NMR spectra is attributed to
a decreasing of the Na – O distances. Therefore, the NMR study tends to demonstrate that the
alkali layers in Li3-xNaxNi2SbO6 compositions do not correspond to an intergrowth of pure Li
and Na layers but do contain both alkaline ions. Indeed, sodium ions present in a Li layer will
increase the local Li-O distance compared to Li3Ni2SbO6 and lithium ions present in the Na
layer will decrease the local Li-O distance compared to Na3Ni2SbO6. Moreover, the overall
broadening of the NMR lines results from a larger distribution of environments as locally
distances and angles will vary depending on the amount of surrounding Li/Na ions. In addition,
it worth noting the decrease of third contribution at 300 ppm in the 7Li spectra with higher
sodium amount. This accounts for less stacking faults for Na-rich compositions, which is logical
when stated that Na3Ni2SbO6 is less sensitive to quenching than Li3Ni2SbO6.
In order to confirm the hypothesis of a random distribution of both lithium and sodium ions in
the same interslab space suggested by the NMR analysis, structural refinements have been
performed on high-resolution XRD and neutron powder diffraction patterns data for the
particular composition Li1.5Na1.5Ni2SbO6. Indeed with four different chemical species (Li, Na,
Ni, Sb) possibly distributed among four crystallographic sites (2d and 4h in the interslab space,
and 2a and 4g in the metal layers), a unique solution cannot be found without i) combining
X-ray with neutrons, that offers a nice contrast (bNi = +10.3 fm, bSb = +5.57 fm, bLi = –1.90 fm,
bNa = +3.63 fm), and ii) imposing some constraints that are detailed as follows. We used as a
starting model the C 2/m monoclinic structural description of Li3Ni2SbO6 by Zvereva et al.27
The total number of Li, Na Ni and Sb was imposed to the nominal composition, with Li and Na
being distributed on the 2d and 4h sites, and Ni and Sb on the 2a and 4g sites. All atomic
positions and the relative occupancy of Li/Na and Ni/Sb were freely refined. An isotropic
The result of the combined XRD/neutron refinement is shown in Figure 4 and the corresponding
table of atomic positions and resulting structure are presented in Table 1 and Figure 5,
respectively. Although the overall Ni/Sb honeycomb pattern is confirmed within the transition
metal slab with 4g and 2a sites mainly occupied by Ni and Sb, respectively; a certain Ni/Sb
mixing is obtained in the structural refinement. Because the relative occupancies of Ni and Sb
were not refined in previous structural refinement, this relative disorder was not reported in
Li3Ni2SbO6 and Na3Ni2SbO6. As stacking faults characterized quenched layered samples, it is
reasonable to assume that the high value of Ni/Sb mixing is over-estimated, as reported for a
similar lamellar compound Li4FeSbO6.28 For comparison, structural refinement for quenched
Li3Ni2SbO6 and Na3Ni2SbO6 from ND also ends up with some Ni/Sb mixing. Interestingly the
Ni/Sb mixing regularly increases from Li3Ni2SbO6 to Na3Ni2SbO6 (Figure S5 and Table S1).
Regarding the interlayer space, the alkali layer is occupied by both lithium and sodium cations
and the refinement indicates a Li/Na mixing very close to the statistical value of 50 %. Lithium
and sodium cations are therefore randomly distributed and seem to not form any kind of
ordering patterns that could be induced by the strong ionic radii difference and/or by the
neighbor Ni/Sb honeycomb-like ordering. To the best of our knowledge, this is the first example
of a complete solid-solution from Li to Na layered oxide with no structural change and no
biphasic domain like for Li1-xNaxNiO2.11–13
A glass-like behavior
After demonstrating the mixing of lithium and sodium despite their very different ionic radii, it
was important to investigate the formation process of this very uncommon crystallographic
thermal treatment. Indeed, a slow cooling rate down to room temperature leads to very different
XRD patterns, with coexistence of Li3Ni2SbO6 and Na3Ni2SbO6 as the main phases and with a
very weak intermediate contribution from the mixed Li3-xNaxNi2SbO6 (see Figure S3 for a
nominal composition “Li1.5Na1.5Ni2SbO6”). In their pioneering investigation on layered Li
1-xNaxNiO2, Matsumura and coworkers also briefly noticed that quenching was mandatory for
obtaining a monophasic product.11 In this current study, we decided to have much deeper grasp
on the details of the stability of the obtained monophasic compositions by combining XRD and
The thermal evolution of quenched Li1.5Na1.5Ni2SbO6 has been monitored by in situ XRD
(Figure 6). At 300 °C, the phase decomposes as its main diffraction peak (001) splits into two
peaks accounting for Li3Ni2SbO6 and Na3Ni2SbO6 domains. At higher temperatures, the
synthesis conditions of a monophasic domain are gathered again and the two peaks merge into
one contribution accounting for (001) of Li1.5Na1.5Ni2SbO6. During the slow cooling down, a
second splitting occurs, showing the reformation of Li3Ni2SbO6 and Na3Ni2SbO6 domains. This
result clearly highlights the role of the final quench for stabilizing at room temperature a
monophasic composition with a random distribution of alkali ions in the interslab layer. Such
thermal feature strongly recalls the behavior of the layered oxide OP4-LixNayCoO2, for which
lithium and sodium are not randomly mixed but alternately ordered one layer over two in
octahedral and prismatic sites, respectively.23
Following the peak position evolution of the Li3Ni2SbO6 and Na3Ni2SbO6 domains can help in
understanding the mechanism involved in the formation of a monophasic domain
Li1.5Na1.5Ni2SbO6 at high temperature. First, it is important to keep in mind the thermal
expansion that significantly increases the slab thickness and thus displaces the (00l) peaks
towards low angles (i.e. from 20.1 ° at room temperature to 19.7 ° at 900 °C for the (001) peak
400 °C to 20.6 °C at 700 °C), whereas the trend is different for the peak related to Na3Ni2SbO6
domains, which slightly shifts to higher angles. The slab thickness contraction (expansion)
accounts for lithium (sodium) diffusion into the Na3Ni2SbO6 (Li3Ni2SbO6) alkali layers, in
agreement with the above NMR analysis (Figure 3). The underlying mechanism consequently
involves a diffusive alkali exchange between domains, respect to a nucleation process for which
only a shift due to thermal expansion would have been observed. The slow cooling monitoring
shows a similar peak splitting and thus confirms that phase decomposition is
thermodynamically favored. To briefly summarize, the Li/Na random distribution mimics an
alkali-glass behavior, however confined within a crystalline matrix.
In parallel, DFT calculations have been performed on about 100 structures with
Li1.5Na1.5Ni2SbO6 stoichiometry, within random ordering of Li/Na in the alkali layer. Figure 7
shows the formation energy of each ordered phase respect to the pure lithiated or sodiated
compounds and the variation of the formation energy as a function of the number of Li-Na
Nearest Neighbor (NN) bonds. As the relative formation energy is positive, all the random
ordered phases are shown to be thermodynamically instable and should decompose following
the equation: Li1.5Na1.5Ni2SbO6 → ½ Li3Ni2SbO6 + ½ Na3Ni2SbO6.
The most stable order consist in the out-of-plane ordered/segregated Li/Na phases (at
~3 meV/atoms) without NN Li-Na, the energy increasing barely linearly with the number of
Li-Na NN bonds. In this situation, the stabilization of any ordered phase does not appear as
feasible except if configuration entropy, thus Li/Na inter-mixing is considered. In fact, the latter
can be evaluated within the Stirling approximation to be ~20 meV/atoms at 900 °C far enough
compared to the relative energy between ordered phases. Consequently, the most probable
hypothesis consists in an entropically stabilized Li/Na intermixing in agreement with the
synthesis conditions and thermal behavior, structural refinement and NMR analysis, and
A complete solid-solution from layered Li3Ni2SbO6 to Na3Ni2SbO6 has been obtained by
conventional solid-state synthesis ended by a final quench. On the transition metal layer, the
honeycomb Ni/Sb cation ordering is maintained all along the solid-solution; however with a
partial Ni/Sb mixing. Focusing on the alkali layer, configuration entropy leads to Li/Na
randomly occupied crystallographic positions.
It is believed that other crystalline transition metal oxides exhibiting 2D confined alkali glass
behavior could now be prepared thanks to a final quenching step, and thus opening the door
towards unexpected physical properties.
The Supporting Information section is available free of charge at DOI: xxx.
The authors declare no competing financial interest.
The authors thank the French National Research Agency (STORE-EX Labex Project
Figure 1. (a) XRD patterns of Li3-xNaxNi2SbO6 compositions obtained after a final quench, (b)
restricted 2θ window to highlight the honeycomb superstructure peaks, and evolution of (c) the monoclinic cell volume and (d) the slab thickness (calculated by c x sin(β)).
Figure 2. Structural hypotheses for the intermediate composition Li1.5Na1.5Ni2SbO6. Nickel and
antimony cations are green and grey, while lithium and sodium cations are in yellow and
Figure 3. Solid-state 7Li and 23Na NMR spectra of as-quenched Li3-xNaxNi2SbO6 compositions,
with blue dotted lines showing the peak shifting from end members (Li3Ni2SbO6 or Na3Ni2SbO6)
to intermediate compositions. The symbol (*) accounts for spinning sidebands.
Figure 4: Combined Rietveld refinement of X-ray (top) and neutron (bottom) diffraction patterns of
Li1.5Na1.5Ni2SbO6. The red crosses, black continuous line and bottom green line represent the observed, calculated, and difference patterns, respectively. Vertical blue tick bars mark the reflection positions.
Figure 5: (a) Structural model for Li1.5Na1.5Ni2SbO6 resulting from the combined X-ray/neutron
Rietveld refinement and (b) in-plane views showing the Ni/Sb and Li/Na intermixing.
Figure 7. (a) Relative formation energy in meV/atom of randomly Na-Li ordered phase respect
to the decomposition in pure Li3Ni2SbO6 + Na3Ni2SbO6 phases. All considered phases are not
stable versus decomposition since they have positive energy. (b) Relative formation energy in
meV/atom as a function of the average number of Na-Li Nearest Neighbor bonds per alkali
ions, showing than as more Na-Li are mixed, as high is the energy of the phase.
Table 1: Structural parameters for Li1.5Na1.5Ni2SbO6, deduced from the combined Rietveld
(1) Shannon, R. D. Revised Effective Ionic Radii and Systematic Studies of Interatomic Distances in Halides and Chalcogenides. Acta Crystallogr. Sect. A Found. Crystallogr.
1976, 32 (5), 751–767. https://doi.org/10.1107/S0567739476001551.
(2) Ng, H. N.; Calvo, C.; Idler, K. L. Crystallographic Studies and Structural Systematics of the C2 c Alkali Metal Metavanadates. J. Solid State Chem. 1979, 27 (3), 357–366. https://doi.org/10.1016/0022-4596(79)90178-6.
(3) Schindler, M.; Hawthorne, F. C.; Alexander, M. A.; Kutluoglu, R. A.; Mandaliev, P.; Halden, N. M.; Mitchell, R. H. Na-Li-[V3O8] Insertion Electrodes: Structures and Diffusion Pathways. J. Solid State Chem. 2006, 179 (8), 2616–2628.
(4) Yuzyuk, Y. I.; Gagarina, E.; Simon, P.; Reznitchenko, L. A.; Hennet, L.; Thiaudière, D. Synchrotron X-Ray Diffraction and Raman Scattering Investigations of (LixNa1-x)NbO3 Solid Solutions: Evidence of the Rhombohedral Phase. Phys. Rev. B - Condens. Matter Mater. Phys. 2004, 69 (14), 1–7.
(5) Mishra, S. K.; Krishna, P. S. R.; Shinde, A. B.; Jayakrishnan, V. B.; Mittal, R.; Sastry, P. U.; Chaplot, S. L. High Temperature Phase Stability in Li0.12Na0.88NbO3: A Combined Powder X-Ray and Neutron Diffraction Study. J. Appl. Phys. 2015, 118 (9), 0–7. https://doi.org/10.1063/1.4929645.
(6) Peel, M. D.; Ashbrook, S. E.; Lightfoot, P. Unusual Phase Behavior in the Piezoelectric Perovskite System, Li <inf>x</Inf>Na<inf>1-X</Inf>NbO<inf>3</Inf>. Inorg. Chem.
2013, 52 (15). https://doi.org/10.1021/ic401061t.
(7) Myung, S. T.; Maglia, F.; Park, K. J.; Yoon, C. S.; Lamp, P.; Kim, S. J.; Sun, Y. K. Nickel-Rich Layered Cathode Materials for Automotive Lithium-Ion Batteries: Achievements and Perspectives. ACS Energy Lett. 2017, 2 (1), 196–223. https://doi.org/10.1021/acsenergylett.6b00594.
(8) Assat, G.; Tarascon, J.-M. Fundamental Understanding and Practical Challenges of Anionic Redox Activity in Li-Ion Batteries. Nat. Energy 2018 2018, 1.
(9) Nayak, P. K.; Erickson, E. M.; Schipper, F.; Penki, T. R.; Munichandraiah, N.; Adelhelm, P.; Sclar, H.; Amalraj, F.; Markovsky, B.; Aurbach, D. Review on
Challenges and Recent Advances in the Electrochemical Performance of High Capacity Li- and Mn-Rich Cathode Materials for Li-Ion Batteries. Adv. Energy Mater. 2018, 8 (8), 1–16. https://doi.org/10.1002/aenm.201702397.
(10) Shilov, G. V.; Nalbandyan, V. B.; Volochaev, V. A.; Atovmyan, L. O. Crystal Growth and Crystal Structures of the Layered Ionic Conductors-Sodium Lithium Titanium Oxides. Int. J. Inorg. Mater. 2000, 2 (5), 443–449. https://doi.org/10.1016/S1466-6049(00)00050-7.
(11) Matsumura, T.; Kanno, R.; Gover, R.; Kawamoto, Y.; Kamiyama, T.; Mitchell, B. J. Synthesis, Structure and Physical Properties of LixNa1-xNiO2. Solid State Ionics 2002,
(12) Holzapfel, M.; De Brion, S.; Darie, C.; Bordet, P.; Chappel, E.; Chouteau, G.; Strobel, P.; Sulpice, A.; Nu?ez-Regueiro, M. D. Decoupling of Orbital and Spin Degrees of Freedom in Li 1-xNaxNiO2. Phys. Rev. B Condens. Matter Mater. Phys. 2004, 70 (13).
(13) Holzapfel, M.; Darie, C.; Bordet, P.; Chappel, E.; Núñez-Regueiro, M. D.; Diaz, S.; De Brion, S.; Chouteau, G.; Strobel, P. Mixed Layered Oxide Phases Na XLi 1-XNiO 2: A Detailed Description of Their Preparation and Structural and Magnetic Identification. Solid State Sci. 2005, 7 (5), 497–506.
(14) Delmas, C.; Fouassier, C.; Hagenmuller, P. Structural Classification and Properties of the Layered Oxides. Phys. B+C 1980, 99 (1?��4), 81–85.
(15) Politaev, V. V; Nalbandyan, V. B.; Petrenko, A. A.; Shukaev, I. L.; Volotchaev, V. A.; Medvedev, B. S. B. Mixed Oxides of Sodium, Antimony (5+) and Divalent Metals (Ni, Co, Zn or Mg). J. Solid State Chem. 2010, 183 (3), 684–691.
(16) Schmidt, W.; Berthelot, R.; Sleight, A. W.; Subramanian, M. A. Solid Solution Studies of Layered Honeycomb-Ordered Phases
O<inf>3</Inf>-Na<inf>3</Inf>M<inf>2</Inf>SbO<inf>6</Inf>(M=Cu, Mg, Ni, Zn). J. Solid State Chem. 2013, 201. https://doi.org/10.1016/j.jssc.2013.02.035.
(17) Ma, J.; Bo, S. H.; Wu, L.; Zhu, Y.; Grey, C. P.; Khalifah, P. G. Ordered and Disordered Polymorphs of Na(Ni<inf>2/3</Inf>Sb<inf>1/3</Inf>)O<inf>2</Inf>: Honeycomb-Ordered Cathodes for Na-Ion Batteries. Chem. Mater. 2015, 27 (7), 2387–2399. https://doi.org/10.1021/cm504339y.
(18) Zvereva, E. A.; Evstigneeva, M. A.; Nalbandyan, V. B.; Savelieva, O. A.; Ibragimov, S. A.; Volkova, O. S.; Medvedeva, L. I.; Vasiliev, A. N.; Klingeler, R.; Buechner, B. Monoclinic Honeycomb-Layered Compound Li 3Ni 2SbO 6: Preparation, Crystal Structure and Magnetic Properties. Dalt. Trans. 2012, 41 (2), 572–580.
(19) Kresse, G.; J. Furthm¨ Uller. Efficient Iterative Schemes for Ab Initio Total-Energy Calculations Using a Plane-Wave Basis Set. Phys. Rev. B 1996, 54 (16), 11169–11186. (20) G.Kresse, D. J. From Ultrasoft Pseudopotentials to the Projector Augmented-Wave
Method. Phys. Rev. B 1999, 59 (3), 1758–1775. https://doi.org/10.1103/PhysRevB.59.1758.
(21) Perdew, J. P.; Burke, K.; Ernzerhof, M. Generalized Gradient Approximation Made Simple. Phys. Rev. Lett. 1996, 77 (18), 3865–3868.
(22) Dudarev, S. L.; Botton, G. A.; Savrasov, S. Y.; Humphreys, C. J.; Sutton, A. P. Electron-Energy-Loss Spectra and the Structural Stability of Nickel
Oxide:  An LSDA+U Study. Phys. Rev. B 1998, 57 (3), 1505–1509. (23) Berthelot, R.; Pollet, M.; Carlier, D.; Delmas, C. Reinvestigation of the
OP4-(Li/Na)CoO2-Layered System and First Evidence of the (Li/Na/Na)CoO2 Phase with OPP9 Oxygen Stacking. Inorg. Chem. 2011, 50 (6), 2420–2430.
(24) Berthelot, R.; Carlier, D.; Delmas, C. Electrochemical Investigation of the P2-Na<inf>x</Inf>CoO<inf>2</Inf>phase Diagram. Nat. Mater. 2011, 10 (1), 74–80. https://doi.org/10.1038/nmat2920.
(25) Blangero, M.; Decourt, R.; Carlier, D.; Ceder, G.; Pollet, M.; Doumerc, J.-P.; Darriet, J.; Delmas, C. First Experimental Evidence of Potassium Ordering in Layered
K4Co7O14. Inorg. Chem. 2005, 44 (25), 9299–9304.
(26) Br?ger, J.; Jiang, M.; Dupr?, N.; Meng, Y. S.; Shao-Horn, Y.; Ceder, G.; Grey, C. P. High-Resolution X-Ray Diffraction, DIFFaX, NMR and First Principles Study of Disorder in the Li2MnO3-Li[Ni1/2Mn1/2]O2 Solid Solution. J. Solid State Chem.
2005, 178 (9), 2575–2585.
(27) Zvereva, E. A.; Evstigneeva, M. A.; Nalbandyan, V. B.; Savelieva, O. A.; Ibragimov, S. A.; Volkova, O. S.; Medvedeva, L. I.; Vasiliev, A. N.; Klingeler, R.; Buechner, B. Monoclinic Honeycomb-Layered Compound Li3Ni2SbO6: Preparation, Crystal Structure and Magnetic Properties. Dalt. Trans. 2012, 41 (2), 572–580.
(28) McCalla, E.; Abakumov, A.; Rousse, G.; Reynaud, M.; Sougrati, M. T.; Budic, B.; Mahmoud, A.; Dominko, R.; Van Tendeloo, G.; Hermann, R. P.; et al. Novel Complex Stacking of Fully-Ordered Transition Metal Layers in Li4FeSbO6 Materials. Chem. Mater. 2015, 27 (5), 1699–1708. https://doi.org/10.1021/cm504500a.
Figure 7 Table 1 Li1.5Na1.5Ni2SbO6 Space Group: C 2/m a = 5.2434(2) Å, b = 9.0997(3) Å, c =5.4034(6) Å, =108.794(8) deg. V = 243.641(5) Å3
Atom Wyckoff site x y z Biso (Å2) Occ
O1 4i 0.736(2) 0 0.209(2) 0.50(6) 1 O2 8j 0.2351(16) 0.1584(9) 0.2230(12) 0.50(6) 1 Ni1/Sb1 4g 0 0.3330(4) 0 0.02(3) 0.882(2) (Ni) 0.118(2) (Sb) Sb2/Ni2 2a 0 0 0 0.02(3) 0.764(2) (Sb) 0.236(2) (Ni) Li1/Na1 4h 0 0.1707(15) ½ 0.48(13) 0.461(8) (Li) 0.539(8) (Na) Li2/Na2 2d 0 ½ ½ 0.48(13) 0.578(8) (Li) 0.422(8) (Na)
XRD: Bragg R-factor = 8.61 %, Rf-factor = 6.23 % Neutrons: Bragg R-factor = 2.81 %, Rf-factor = 2.30 %